Solid State Structure of Bi(N3)3, Bi(N3)3.Solvates and the Structural Dynamics in the [Bi(N3)6]3- Anion
Kati Rosenstengel; Axel Schulz; Alexander Villinger; Inorganic Chemistry 52 (2013) 6110–6126; doi:10.1021/ic400493v

data_4334936
_publ_contact_author_address
;
Universit\"at Rostock
Institut f\"ur Chemie
Abteilung f\"ur Anorganische Chemie
Albert-Einstein-Strasse 3a 
18059 Rostock
Bundesrepublik Deutschland
;
_publ_contact_author_email
;
axel.schulz@uni-rostock.de, alexander.villinger@uni-rostock.de'
;
_publ_contact_author_fax         '+49 (0)381/498-6382'
_publ_contact_author_name        'Axel Schulz, Alexander Villinger'
_publ_contact_author_phone       '+49 (0)381/498-6400 or 6403'
_publ_section_title
;
 Solid State Structure of Bi(N3)3, Bi(N3)3.Solvates and the Structural
 Dynamics in the [Bi(N3)6]3- Anion
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              6110
_journal_page_last               6126
_journal_paper_doi               10.1021/ic400493v
_journal_volume                  52
_journal_year                    2013
_chemical_formula_moiety         '3(C24 H20 P +), Bi N18 3-'
_chemical_formula_sum            'C72 H60 Bi N18 P3'
_chemical_formula_weight         1479.27
_chemical_name_systematic
;
 ?
;
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_Int_Tables_number      14
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_author_name               'Villinger, A.; Rosenstengel, K.'
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 96.8590(10)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   13.3072(2)
_cell_length_b                   22.6362(4)
_cell_length_c                   21.9663(3)
_cell_measurement_reflns_used    9769
_cell_measurement_temperature    153(2)
_cell_measurement_theta_max      54.416
_cell_measurement_theta_min      4.894
_cell_volume                     6569.43(18)
_diffrn_ambient_temperature      153(2)
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measurement_device_type  'Bruker-Nonius Apex X8-CCD-diffractometer'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0499
_diffrn_reflns_av_sigmaI/netI    0.0521
_diffrn_reflns_limit_h_max       19
_diffrn_reflns_limit_h_min       -20
_diffrn_reflns_limit_k_max       34
_diffrn_reflns_limit_k_min       -28
_diffrn_reflns_limit_l_max       33
_diffrn_reflns_limit_l_min       -30
_diffrn_reflns_number            119781
_diffrn_reflns_theta_full        32.60
_diffrn_reflns_theta_max         32.60
_diffrn_reflns_theta_min         1.30
_exptl_absorpt_coefficient_mu    2.816
_exptl_absorpt_correction_T_max  0.8720
_exptl_absorpt_correction_T_min  0.4477
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   '(SADABS; Sheldrick, 2004)'
_exptl_crystal_colour            yellow
_exptl_crystal_density_diffrn    1.496
_exptl_crystal_description       block
_exptl_crystal_F_000             2984
_exptl_crystal_size_max          0.34
_exptl_crystal_size_mid          0.23
_exptl_crystal_size_min          0.05
_refine_diff_density_max         2.346
_refine_diff_density_min         -2.751
_refine_diff_density_rms         0.093
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.006
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     903
_refine_ls_number_reflns         23903
_refine_ls_number_restraints     9
_refine_ls_restrained_S_all      1.006
_refine_ls_R_factor_all          0.0717
_refine_ls_R_factor_gt           0.0369
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0178P)^2^+6.3368P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0609
_refine_ls_wR_factor_ref         0.0700
_reflns_number_gt                16681
_reflns_number_total             23903
_reflns_threshold_expression     >2\s(I)
_cod_data_source_file            ic400493v_si_002_13.cif
_cod_data_source_block           kr11_2_153K
_cod_original_sg_symbol_H-M      'P 21/n'
_cod_database_code               4334936